QB/T 1619-2018 English PDF (QBT1619-2018)
QB/T 1619-2018 English PDF (QBT1619-2018)
QB/T 1619-2018: Wallet
LIGHT INDUSTRY STANDARD OF
THE PEOPLE’S REPUBLIC OF CHINA
Classification number. Y48
Registration number. 63688-2018
Replacing QB/T 1619-2006
ISSUED ON. MAY 08, 2018
IMPLEMENTED ON. SEPTEMBER 01, 2018
Issued by. Ministry of Industry and Information Technology of PRC
Table of Contents
Foreword ... 3
1 Scope ... 5
2 Normative references ... 5
3 Terms and definitions ... 6
4 Product classification ... 7
5 Requirements ... 7
6 Test methods ... 10
7 Inspection rules ... 11
8 Marking, packaging, transport and storage ... 12
Appendix A (Informative) Common wallet and part schematics ... 14
Appendix B (Normative) Test methods for color fastness to rotatory rubbing . 15 Appendix C (Normative) Special type test ... 18
This standard specifies the terms and definitions, product classification, requirements, test methods, inspection rules, markings, packaging,
transportation and storage of wallet.
This standard applies to all kinds of wallet which are made from leather, fur, artificial leather/synthetic leather, regenerated leather, textile, and so on. The cellphone cover may make reference to it.
2 Normative references
The following documents are essential to the application of this document. For the dated documents, only the versions with the dates indicated are applicable to this document; for the undated documents, only the latest version (including all the amendments) are applicable to this standard.
GB/T 251 Textiles - Tests for color fastness - Grey scale for assessing staining
GB/T 2912.1 Textiles - Determination of formaldehyde - Part 1. Free and hydrolyzed formaldehyde (water extraction method)
GB/T 17592 Textiles - Determination of the banned azo colorants
GB 19340 Adhesives for footwear and case and bag
GB/T 19941 Leather and fur - Chemical tests - Determination of
GB/T 19942 Leather and fur - Chemical tests - Determination of banned azo colorants
GB 20400 Leather and fur - Limit of harmful matter
GB 21550 The restriction of hazardous materials in polyvinyl chloride
GB/T 22889 Leather - Physical and mechanical tests - Determination of
surface coating thickness
The fittings that have open/close function.
The metal mouth inlayed at the opening.
4 Product classification
4.1 It is classified into the wallets made from leather, fur, regenerated leather, artificial leather/synthetic leather, textile and other materials by the surface layer material.
4.2 It is classified into frame wallet, suit wallet, wallet, certificate wallet, key case, name card holder, and so on (the common wallet and part schematics are as shown in Appendix A) by types.
5.1 Raw materials and fittings
It is selected in accordance with relevant product standards.
5.2 Limit of harmful substance
The limit of harmful substance of leather, fur, regenerated leather, and textile material shall comply with the provisions of Table 1, the limit of harmful substance of PVC artificial leather shall comply with the provisions of GB 21550, the limit of harmful substance of adhesives used in wallet shall comply with the provisions of Table 2.
Table 1 -- Limit of harmful substances of leather, fur, regenerated leather, and textile materials
In milligram per kilogram
Item Limit value
Free formaldehyde, ≤ 75
Decomposable harmful aromatic amine dye, ≤ 30
Note. The name of the forbidden aromatic amine is as shown in Appendix A in GB 20400. If the content of the 4-aminobiphenyl and 2-aniline exceeds 30 mg/kg, and there is no other evidence, it cannot judge whether the forbidden azo dye is used based on the currently available knowledge. one test, totally 200 tests are performed, respectively.
6.5 Zipper durability
Select 20 cm length zipper to perform test at the frequency of (20 ± 1) time/min, one opening plus one closing form one test, totally 200 tests are made. If the zipper length is less than 20 cm, perform test within the maximum length range of the zipper.
6.6 Hardware fitting corrosion resistance
It is tested in accordance with QB/T 3826 (excluding riveted piece, metal chain tooth), the test time is 16 h. Only the zipper pull of the zipper head is evaluated. 7 Inspection rules
The products of the same type and same specification which are produced by the same type of raw materials in accordance with the same production process form one inspection batch.
7.2 Exit-factory inspection
Each batch of products shall be subject to appearance inspection one by one, which can only be exit-factory after being inspected and qualified.
7.3 Conventional type inspection
Under one of the following cases, it shall randomly take 3 products from those which passes exit-factory inspection for conventional type inspection.
a) In case of major change of product structure, process, and material; b) In case of production restoration after 6-month suspension;
c) In case of national quality technical supervision institute proposes type inspection;
d) In case of normal production, at least 1 type inspection is made every 6 months.
7.4 Special type inspection
It is performed in accordance with the provisions of Appendix C.
7.5 Decision rules
Test methods for color fastness to rotatory rubbing
B.1 Test environment
The specimen shall be placed in a standard environment of temperature (20 ± 2) °C and relative humidity (65 ± 4)% for conditioning for at least 24 h, the test shall also be performed at this temperature and humidity conditions.
B.2 Test instrument and material
B.2.1 Rotatory rubbing testing machine
It shall contain the following parts.
- Test bench (preferably metal), which can fix the specimen;
- Vertical rotatory shaft, which is used to fix the circular felt, the rotation speed is (150 ± 5) r/min;
- Apply the (24.5 ± 0.5) N or (7.1 ± 0.2) N to the rotating circular felt; - Counter.
B.2.2 Test material
Circular combed felt, with holes at middle part, which shall comply with the following requirements.
- Outer diameter (25 ± 1) mm, inner diameter (3.0 ± 0.5) mm;
- Thickness, which is measured in accordance with the provisions of Table B.1;
- Density (190 ± 20) kg/m3.
Table B.1 -- Felt thickness test method
Thickness/mm Downward pressure/pressure foot size Sample
6.5 ± 0.5 (49 ± 5) kPa/(10 ± 1) mm Cut felt or sheet material not cut
5.0 ± 0.5 (2.0 ± 0.2) kPa/(19 ± 10) mm Cut felt
B.3 Specimen preparation
The requirements are as follows.
- When the sample can be flatly fixed onto the test bench, it may directly use the sample to perform test;
- When the sample cannot be flatly fixed onto the test bench, cut a strip specimen of 30 mm x 90 mm from the sample surface layer material to
Test shall be performed on parts free from stitching lines or holes.
B.4.1 Dry rubbing test
B.4.1.1 Fix the specimen onto the test bench, apply the load, to make the test head pressure reach to (24.5 ± 0.5) N.
B.4.1.2 Fix the felt onto the test machine shaft.
B.4.1.3 Lower down the rotating shaft, to make the felt contact to the specimen, select the number of rotations in accordance with Table B.2, start the instrument. B.4.1.4 After the test, rise the rotating shaft, take off the specimen and felt, use the grey scale as specified in GB/T 251 to assess the staining grade of the felt. B.4.2 Wet rubbing test
B.4.2.1 Weight the mass of dry felt, place the dry felt into the grade III water or deionized water, slowly heat it to boiling, keep boiling for 60 s, pour off hot water, replace fresh water, to make the circular felt cool to room temperature, take the felt off water, place it in between 4 water absorbent papers (2 above and 2 below, with the test surface in contact with the filter paper horizontally), place a (900 ± 10) g load onto the filter paper, keep it for about 1 min, gently extrude the circular felt to adjust its moisture, weigh it to make the wet felt mass reach to (3.0 ± 0.3) g, the immersion time of the circular felt in water shall not exceed 24 h.
B.4.2.2 Fix the specimen onto the test bench, make the test head pressure be (7.1 ± 0.2) N.
B.4.2.3 Fix the wet felt onto the test machine shaft.
B.4.2.4 Lower down the rotating shaft, to let the felt contact the specimen, select the number of rotations in accordance with Table B.2, start the instrument. B.4.2.5 After the test, rise the rotating shaft, take off the specimen and felt, naturally dry the felt at room temperature, use the grey scale as specified in GB/T 251 to assess the staining grade of the felt.